new jou rnal of ph ys ics - radboud the open access journal for physics new jou rnal of ph ys ics
Post on 08-Jan-2020
Embed Size (px)
T h e o p e n – a c c e s s j o u r n a l f o r p h y s i c s
New Journal of Physics
STM studies of the self-assembly of manganese porphyrin catalysts at the Au(111)−n-tetradecane interface
Bas Hulsken1, Johannes A A W Elemans1,3, Jan W Gerritsen1, Tony Khoury2, Maxwell J Crossley2, Alan E Rowan1, Roeland J M Nolte1 and Sylvia Speller1 1 Institute for Molecules and Materials, Radboud University Nijmegen, Toernooiveld, 6525 ED Nijmegen, The Netherlands 2 School of Chemistry, University of Sydney, NSW 2006, Australia E-mail: J.Elemans@science.ru.nl
New Journal of Physics 11 (2009) 083011 (14pp) Received 6 January 2009 Published 12 August 2009 Online at http://www.njp.org/ doi:10.1088/1367-2630/11/8/083011
Abstract. The precise structure of monolayers of catalytic manganese porphyrins at the interface of an Au(111)-surface and an n-tetradecane liquid has been determined in a liquid-cell scanning tunneling microscope (STM). Before the addition of the manganese porphyrins, an ordered monolayer of lamellae of n-tetradecane molecules on the Au(111) surface could be imaged. It was found that only domain boundaries in this monolayer were correlated to the underlying gold surface, but not the orientation of the n-tetradecane lamellae and the molecules within them. Both the reconstruction of the Au(111) surface and the ordering of the first layer of n-tetradecane can direct the ordering of the manganese porphyrins that are subsequently added to the liquid phase.
3 Author to whom any correspondence should be addressed.
New Journal of Physics 11 (2009) 083011 1367-2630/09/083011+14$30.00 © IOP Publishing Ltd and Deutsche Physikalische Gesellschaft
1. Introduction 2 2. Experimental 3
2.1. STM setup . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 2.2. Preparation of the Au(111) surface . . . . . . . . . . . . . . . . . . . . . . . . 3 2.3. Preparation of the n-tetradecane liquid . . . . . . . . . . . . . . . . . . . . . . 3 2.4. STM topography measurements . . . . . . . . . . . . . . . . . . . . . . . . . 4 2.5. Correlation methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4
3. Results and discussion 6 3.1. Structure of the Au(111)/n-tetradecane interface . . . . . . . . . . . . . . . . 6 3.2. Self-assembly of manganese porphyrins at the Au(111)−n-tetradecane interface 9
4. Conclusions 13 Acknowledgments 13 References 13
While many conventional spectroscopic techniques are available to study reaction mechanisms at the ensemble level, it is only recently that fluorescence microscopy has been applied to monitor, by single turnover counting, chemical reactions carried out on crystal faces  and by enzymes . With the advent of scanning probe microscopy, it has become possible to image chemical reactions even down to the atomic level, albeit under idealized conditions . During the past few years, we have developed a highly sophisticated STM setup equipped with an inert liquid cell and a bell jar that can be filled with any gas desired. Using this equipment, surfaces can be studied at solid–liquid interfaces under very clean conditions, comparable to those in ultrahigh vacuum (UHV) . Currently, one of the most appealing challenges of scanning probe research is to go beyond just the imaging of molecules, and to study dynamic processes that occur at the chemically highly relevant environment of a solid–liquid interface . In particular, studying chemical reactions at such an interface is highly interesting, since it resembles the environment in which most chemical reactions in academic and industrial laboratories take place. In a liquid-cell STM, we have very recently succeeded for the first time to image at a solid–liquid interface a multi-step catalytic oxidation reaction at the single catalyst level . Manganese(III) porphyrin catalysts Mn1 (figure 1) were immobilized flat at the interface of an Au(111) surface and an n-tetradecane solution, and the resulting catalytic monolayer appeared highly active in oxidizing alkene molecules, which were added to the liquid phase, into epoxides. During the course of the catalytic studies, we became aware of the essential role that the solid–liquid interface seems to play with respect to the ordering and the catalytic performance of the porphyrin monolayer. For example, we suspected a prominent role of the gold surface in binding to the manganese metal in the center of the porphyrins, because under the same conditions porphyrins that do not contain a metal center were found not to adsorb to the same solid–liquid interface . For this reason it was our aim to investigate in high detail the nature of the interface between Au(111) and n-tetradecane, and the subsequent
New Journal of Physics 11 (2009) 083011 (http://www.njp.org/)
Figure 1. Molecular structure of manganese porphyrin catalyst Mn1.
adsorption of Mn1 porphyrins to this interface. Here we report detailed STM studies of these investigations, which will demonstrate that a monolayer of adsorbed n-tetradecane molecules can influence the subsequent ordering of the porphyrins, and that this ordering is also influenced by the reconstruction present on the Au(111) surface.
2.1. STM setup
The liquid-cell STM setup was home-built based on earlier designs [4, 8]. The liquid cell was made of an inert polymer (Kel-F) and the electrode for the sample bias voltage of platinum. The sample holder was made out of gilded steel, and held in place by a magnet outside of the liquid cell. The entire STM was placed under a bell jar, which can be flushed with argon or oxygen.
2.2. Preparation of the Au(111) surface
Au(111) surfaces were prepared by evaporating 99.99% gold on freshly cleaved mica. The gold was grown epitaxially on the heated mica (< 300 ◦C), at a pressure of 10−7 mbar, and annealed for 2 h at 300 ◦C at a pressure of 10−8 mbar. It was found that the quality of the gold films deteriorated quickly, and therefore gold films no older than 2 days were used in the present study. Just before mounting the film in the liquid cell it was annealed in a hydrogen flame.
2.3. Preparation of the n-tetradecane liquid
n-Tetradecane was purchased from Aldrich and twice distilled under reduced pressure before use. It was purged extensively (>12 h) with argon prior to the STM experiment to ensure the removal of any other gases dissolved in the liquid.
New Journal of Physics 11 (2009) 083011 (http://www.njp.org/)
2.4. STM topography measurements
STM measurements were performed in a home-built liquid-cell STM connected to an Omicron SCALA SPM controller. STM tips were mechanically cut from platinum–iridium (80–20) wire. All STM images presented are constant current images, typically applying a very low tunneling current of around 10 pA, and have been corrected for background slope (by subtracting a plane). In all cases, the bias voltage was applied to the Au(111) surface. Some spike noise was removed by filtering the data through a median filter with a [3 × 3] pixel filter size (only the STM images in figure 2).
2.5. Correlation methods
A crystalline surface is an endless repetition of one unique unit cell; one can reason that an STM image of an n unit cell large area of a crystalline surface is equivalent to n STM images of a 1 unit cell large area. In this paper, the positions of the individual unit cells were determined by performing a correlation between a manually selected part of the STM image, which contains at least one unit cell, and the complete STM image . The correlation averaging procedure will be explained here by a relatively simple model system, i.e. a monolayer of non-symmetric organic molecules on a graphite surface (figures 2(A) and (B)). First, a small reference area, containing at least one unit cell, is selected manually in an STM image of the monolayer (figure 2(C)). The filter program then searches, by means of correlation, the entire STM image for areas equivalent to the selected reference area. Subsequently, the found areas are sorted by their degree of similarity to the reference area, which is quantified by the correlation coefficient. Which of the found areas are similar enough to the reference area to be used for the correlation averaging procedure can usually be readily established by identifying the correlation maxima and the distribution of the equivalent areas found over the STM image in an intermediate correlation map (figure 2(E)). This identification, which is the second interactive step in the correlation averaging procedure, allows for the localization and subsequent extraction of n different STM sub-images, which are situated at a grid with the same spacing as the unit cells. This division in sub-images is used for two things: firstly, by averaging the n different sub- images, an STM image with the size of the sub-image is obtained with a sqrt(n) reduction in noise (cf figure 2(D)); and secondly, because the positions of the unit cells in the original STM image, as found by the correlation method, represent the crystal lattice, an accurate measurement of the unit cell’s dimensions can be obtained. For the noise reduction, the sub- images used for the averaging are replaced by the averaged sub-image in the original STM image (figure 2(F)).
In addition to a reduction in noise and enhanced resolution, the correlation method offers another important use: it can provide quantitative information about the errors in the measurement of distance